electrically conductive adhesives (ecas) contents .1 electrically conductive adhesives (ecas) james
Post on 09-Sep-2018
Embed Size (px)
Electrically Conductive Adhesives (ECAs)
James E. Morris (firstname.lastname@example.org) Department of Electrical & Computer Engineering, Portland State University, Oregon, USA
Johan Liu (email@example.com) Department of Production Engineering, Chalmers University of Technology, Goteborg, Sweden
I. Introduction A. Technology Drivers B. Isotropic Conductive Adhesives (ICAs) C. Anisotropic Conductive Adhesives (ACAs) D. Non-Conductive Adhesive (NCA.) II. Structure
A. ICA B. ACA C. Modelling III. Materials and Processing
A. Polymers B. ICA Filler C. ACA Processing
IV. Electrical Properties A. ICA
1. Percolation theory 2. Inter-particle conduction 3. Intra-particle resistance 4. Contact resistance
B. Electrical Measurements C. ACA
V. Mechanical Properties A. ICA
B. ACA VI. Thermal Properties
A. Thermal Characteristics B. Maximum Current Carrying Capacity
VII. Reliability A. ICA
1. Cure schedule 2. Moisture effects 3. Galvanic corrosion 4. Thermo-mechanical
B. ACA C. General Comments VIII. Environmental Impact IX. Further Study X. References
I. Introduction A. Technology Drivers There are two primary categories of Electrically Conductive Adhesive (ECA): Isotropic Conductive Adhesive (ICA) Anisotropic Conductive Adhesive (ACA). ACAs are available as paste (ACP) or film (ACF).
Both types conduct through metal filler particles in an adhesive polymer matrix. ECAs have been used for electronics packaging applications for decades in hybrid, die-attach and display
assembly. ICAs have been used extensively for die attach, and in automotive electronics. ACF technology is employed with almost every liquid crystal display. But there has been growing interest from the electronics industry over the past decade or so in other kinds of electronics packaging applications. While toxicity issues and environmental incompatibility of the lead in tin-lead solders triggered that greater interest at the outset, it has been the other evident advantages which continue to drive further research. ECAs can offer the following additional potential advantages: Fine-pitch capability, especially when using ACAs for flip-chip Elimination of underfilling with ACA bonding; Low temperature processing capability; Flexible, simple processing and hence low cost.
In addition, solder failures due to the formation of voids or brittle intermetallics are controlled by diffusion rates at small dimensions, and time-to-failure scales as the square of the dimensions, limiting solder reliability lifetimes at ultra-fine pitch .
ACF has long been the interconnect of choice in the LCD display industry, and ACP is now finding applications in flex circuits and surface mount technology (SMT) for chip-scale package (CSP), ASIC, and flip chip attachment for cell phones, radios, PDAs, laptop PCs, and cameras. ICAs are used extensively in die-attach, for many years for small passive chip attachment in automotive electronics, and in varied consumer products, e.g. in Matsushita/Panasonics stud bump joints. More recent applications include RFID tags, potentially for the antenna as well as chip connections.
This chapter presents an overview of the current status of understanding of conductive adhesives in various electronics packaging applications, and of some fundamental issues relevant to their continuing development. It is organized with initial discussions of basic ECA concepts of structure-related properties, and how these are affected by material selection and processing, followed by general properties and reliability considerations. In each section, there is material common to both ICAs and ACAs, and parallel treatments of topics specific to each.
B. Isotropic Conductive Adhesives (ICAs) Ag is usually used as the filler material due to its high conductivity and simple processing for ICA applications. Figure 1 shows the microstructure of an ICA joint, (a) in schematic form, (b) for a flip chip component, and (c) for SMT attachment, (both on FR-4 substrates.) The metallic filler content is high enough (between 25-30 volume percent) to cause direct metallic contact from bump or lead to circuit board pad. C. Anisotropic Conductive Adhesives (ACAs) Polymer based metal-plated spheres or Ni fillers are mainly used for ACA applications. In an ACA joint, the filler particles normally constitute between 5-10 volume percent, and do not cause any direct metallic contact. It is only after the application of pressure during curing that electrical conduction becomes possible in the normal (z-axis) direction, as is illustrated in Figure 2. The Ni particles are usually matched to soft Au contacts, and the contact deforms to define the contact area. By contrast, the polymer beads, usually Au-plated, deform to establish bump and pad contacts. As there is no direct contact between the particles, ACA technology is very suitable for fine pitch assembly, and is starting to find applications in flip-chip technology.
D. Non-Conductive Adhesive (NCA.)
The complementary NCA technology is mentioned only briefly here, for completeness. In this case, the contacts themselves are in direct metal-to-metal contact, held together by the NCA. The concept relies upon surface asperities for the direct contacts.
A. ICA As the proportion of metal in the ICA polymer matrix is increased, (Figure 3,) the resistance drops only slightly until the percolation threshold is reached, when the first continuous metal path is established through the composite material . The resistance continues to drop more slowly as multiple parallel paths are developed with the continued addition of more metal filler. Ideally one would like to use the minimum quantity of filler necessary to pass the threshold, but in practice manufacturing tolerances require a design target composition significantly beyond the threshold. Very small contact volumes increase the statistical spread of resistivities already inherent in a percolation structure. Minimal filler content is a requirement for both economic reasons (since Ag is expensive) and to maximize the proportion of polymer adhesive. Both issues can be addressed by the use of metal flakes (or rods) as filler instead of spheres. The benefits can be readily understood by considering the extreme case of flakes of zero thickness, which would clearly establish a percolation threshold at zero metal content, i.e. at 100% adhesive with zero filler cost. Practical commercial materials achieve substantial reduction in the threshold composition by the use of flakes, by virtue of the increased connectivity which accompanies the increased surface-to-volume ratio, compounded by bi-modal particle size distributions (Figure 4.) The efficacy of bi-modal particle distributions has been demonstrated  and either flakes or powders can be used for the smaller particles .
Theoretical simulation has been carried out to optimize the electrical performance of a conductive adhesive joint using a bimodal distribution of metal fillers using computer modeling with finite-element analysis. Two classes of metal fillers were used, i.e. nano-scale and micro-scaled particles. The goal was to decrease the metal loading to improve the mechanical performance for specified electrical properties. It has been shown that it is possible to decrease the total metal loading with good electrical conductivity using a bimodal filler distribution , but that the nano-particles increase resistivity for a given total filler content, due to mean free path limits and increased numbers of contacts.
In addition, the flakes at the material surfaces seem to be aligned parallel to the surface to a depth of a few flake thicknesses (Figure 4.) The effect seems to be universal, with squeegee or syringe dispensation, and also appears inside air bubbles, probably due to surface tension . One also sees particle alignment inside the material, parallel to the contacts, if pressure is applied , as seen in Figure 1(b). Particulate orientations are important for predictions of both adhesive strength and electrical resistance. Flow modeling of the ICA under stencil, print, or dispensation, and/or positioning pressure is much more difficult than underfill flow modeling  due to filler sizes and shapes. Recently, a dynamic model of the effects of compression has demonstrated flake alignment quite dramatically .
There are various novel approaches to the improvement of electrical connectivity at a given metal content, including magnetic alignment of nickel filler rods , the use of polymer particles to force z-axis alignment of flakes , and electric fields . Anything that increases the packing density/efficiency of the particles also increases the connectivity and reproducibility of the structure, permitting the design composition to move closer to the percolation threshold, and a reduction in metal filler.
Modelling of the material structure for prediction of the electrical properties has included Distributions of uniformly sized spheres  2D  and 3D  rectangular particles with limited size distributions and x, y, z orientations Rectangular particles rotated about the x, y, z axes in 1 increments . The extension to bimodal flake representations requires a dramatic increase in computing power. The difficulty lies in the development of an efficient algorithm for the random placement of the particles, which must not impinge upon the space occupied by another. As the structure fills up, this process becomes more and more time consuming. A potential energy technique has proved effective , but the most recent advances have been by the use of compression